- Nano Express
- Open Access
Reduced Graphene Oxide-Coated Si Nanowires for Highly Sensitive and Selective Detection of Indoor Formaldehyde
Nanoscale Research Letters volume 14, Article number: 97 (2019)
Although significant developments have been made in the low-concentration formaldehyde monitoring in indoor air by using gas sensors, they still suffer from insufficient performance for achieving ppb-level detection. In this work, <100> oriented Si nanowires (SiNWs) with high specific surface area were prepared via metal-assisted chemical etching method (MACE), and then were uniformly coated with graphene oxide (GO) followed by the subsequent reductive process in H2/Ar atmosphere at 800 °C to obtain reduced graphene oxide (RGO). The RGO coating (RGO@n-SiNWs) obviously enhances SiNWs sensitivity to low-concentration formaldehyde, benefiting from the increased specific surface area, the sensitization effect of RGO, and the formation of p-n junction between SiNWs and RGO. Specifically, RGO@n-SiNWs exhibits a high response of 6.4 to 10 ppm formaldehyde at 300 °C, which is about 2.6 times higher than that of pristine SiNWs (~ 2.5). Furthermore, the RGO@n-SiNWs show a high response of 2.4 to 0.1 ppm formaldehyde which is the largest permissive concentration in indoor air, a low detection limit of 35 ppb obtained by non-linear fitting, and fast response/recovery times of 30 and 10 s. In the meanwhile, the sensor also shows high selectivity over other typical interfering gases such as ethanol, acetone, ammonia, methanol, xylene, and toluene, and shows a high stability over a measurement period of 6 days. These results enable the highly sensitive, selective, and stable detection of low-concentration formaldehyde to guarantee safety of indoor environment.
Nowadays, as one of the toxic volatile organic compounds (VOCs) in newly built house environment, formaldehyde (HCHO) is seriously threatening human health [1,2,3,4,5,6,7,8,9,10,11,12], which is considered to be one of the major sources of sick building syndrome (SBS) [13, 14], and a carcinogen by International Agency for Research on Cancer (IAIC) . Therefore, several standards have been set up to avoid the risk induced by the pollution of indoor air. In the literatures, the upper limit of formaldehyde concentration established by the National Institute for Occupational Safety and Health (NIOSH) is 0.1 ppm in the living room and 1 ppm in industrial production workshop . Meanwhile, the World Health Organization (WHO) also established a safe standard of 0.08 ppm averaged over 30 min for long-term exposure in formaldehyde vapor . Therefore, the successful detection of low-concentration HCHO makes a great stride to ensure the safety of living environment.
Although many schemes have been developed for detecting low-concentration HCHO, including liquid chromatograph (LC) [16, 17], spectroscopy , etc., these techniques have limitations for portable use and real-time monitoring due to their bulky sizes and complicated analysis processes . Currently, gas sensors based on the semiconductor nanostructures (e.g., In2O3 [19, 20], Cr2O3 , SnO2 [21,22,23]) are extensively employed in the detection of low-concentration HCHO, owing to their high sensitivity, fast response, and excellent chemical stability [2, 10, 19, 24,25,26,27,28,29,30,31,32]. These sensors based on semiconductor nanostructures offer significant advantages compared with LC and spectroscopy, such as easy miniaturization for portable use, low cost, and in-situ detection. However, their responses to HCHO need to be further improved at the ppb level though they are good at ppm level. For example, Chen et al. reported Ga-doped In2O3 nanofiber sensors which showed a high response (defined as Ra/Rg, where the Ra and Rg are the resistances of the sensor in air and in HCHO) of 52.4 to 100 ppm HCHO, while < 1.5 to 0.1 ppm, which needs to be enhanced to meet the response requirement of practical utilization limitation of Ra/Rg = 2 . Therefore, it is an urgent affair to find an efficient route to enhance the sensitivity for reaching the safe detection limitation. Silicon nanowires (Si NWs) have been selected as one of semiconductor materials to be used in chemical sensors. For example, biosensors based on chemically modified Si NW field effect transistors have been reported and demonstrated a superior sensitivity and selectivity to proteins . However, this sensor fabrication needs a high cost and complicated process as the sensitivity has to be improved by the filed effect.
Recently, the incorporation of graphene with nanostructured semiconductor gas sensors becomes a promising approach to improve the sensitivity, due to its high specific surface area and exceptional sensitivity to gases . Compared with the sensitization effect of conventional noble metals (e.g., Pt, Pd, and Au nanoparticles) [35,36,37], this strategy can not only possess the merits of low cost and high efficiency but also enlarge the surface area and improve the electron transport. For example, reduced graphene oxide (RGO)-SnO2 , RGO-Cu2O , graphene-SnO2  have demonstrated excellent enhancement of gas sensitivity. However, many reports put the semiconductor nanostructures on the surface of RGO or graphene to form simple contact, of which the efficient contact area is too restricted to achieve the maximization of sensitivity. Therefore, it is significant to search an efficient and feasible strategy to realize core-shell structures based on RGO and semiconductor.
In this work, highly sensitive and selective detection of low-concentration HCHO was achieved by a core-shell structure of RGO-coated silicon nanowires (SiNWs), with increased specific surface area twice as large as SiNWs. Specifically, the response of reduced graphene oxide-coated n-type silicon nanowires (RGO@n-SiNWs) increases about 2.6× toward 10 ppm HCHO (~ 6.4) than that of pristine SiNWs (~ 2.5) at the best operation temperature of 300 °C, which is attributed to the excellent sensitization effect of RGO. The as-fabricated sensors can reach a superior application detection limitation of as low as 35 ppb, and the response/recovery times are as fast as 30/10 s. Besides the improved sensitivity, the selectivity is high over typical interfering gases (e.g., ethanol, acetone, ammonia, methanol, xylene, and toluene) and the stability is good in a period of 6 days. All of the results made a significant stride toward using reduced graphene oxide-coated silicon nanowires (RGO@SiNWs) for the low concentration HCHO detection in indoor environment.
Materials and Methods
Fabrications of SiNWs Arrays
n (100) and p (100) Silicon wafers (0.005–0.02 Ωcm and 0.001–0.005 Ωcm) were employed as starting wafers (3.0 cm × 3.0 cm). Before the etching process, the Si wafers were cleaned in acetone for 10 min, ethanol for 10 min, and deionized (DI) water for 10 min in turn. The cleaned starting wafers were immersed in oxidant solution containing H2SO4 (97%, Sigma-Aldrich) and H2O2 (35%, GR 30 wt.% in H2O, Aldrich) in a volume ratio of 3:1 for 30 min to remove the organic contaminants on the surface. After the cleaning step, the samples were then immersed into 5% HF solution for 8 min at room temperature to dissolve the thin oxide layer formed on the surface and thus the fresh Si surfaces were H-terminated. Next, the cleaned Si wafers were immediately transferred into an Ag coating solution containing 0.005 M AgNO3 (99.99%, Aladdin) and 4.8 M HF (Aladdin, GR 40%), which was slowly stirred for 1 min at room temperature (~25 oC). After a uniform layer of Ag nanoparticles (AgNPs) was deposited on the surfaces, the AgNPs-coated wafers were washed with deionized water to remove the extra Ag+ ions. Then, the wafers were etched in the etching solution (H2O2 = 0 .4 M and HF = 4 .8 M) for 30 min at room temperature in the dark. Finally, the samples were dipped in the aqueous solution of HNO3 (70%, Sigma-Aldrich) to dissolve the Ag catalyst, and then rinsed with deionized water for several times to remove residual layer. The fabricated SiNWs were slowly scraped by a sharp blade.
SiNWs Functionalized with RGO
The graphene oxide (GO) dispersion was synthesized by the modified Hummer’s method , and then was ultrasonically dispersed in 60 mL DI water for 3 h to prepare the GO solution (30 mg). In a typical synthesis, the obtained SiNWs (0.2 g) were firstly dispersed in the mixture of DI water (10 mL) and ethanol (30 mL), then ethylenediamine (400 μL) was dropwise added. After the ultrasonic treatment for 20 min, 20 mL GO solution was added to the above solution and kept vigorous stirring. Subsequently, the product was collected by centrifugation and washed with ethanol for several times, then dried at 60 °C to obtain GO@SiNWs. Finally, the GO@SiNWs was reduced in H2/Ar atmosphere at 800 °C (2 °C min−1) to obtain RGO@SiNWs.
Characterization of SiNWs and RGO@SiNWs
The morphology of SiNWs and RGO@SiNWs was observed by scanning electron microscopy (SEM, JSM-7001F+INCA X-MAX) and transmission electron microscopy (TEM, JEM-2100F). Besides, the crystal structure was studied by X-ray diffraction (XRD, X’Pert PRO MPD). Additionally, in order to analyze the surface area and pore size distribution, nitrogen absorption-desorption isotherm was performed on a specific area and a pore-size analyzer (SSA-7300, BUILDER) by the Brunauer–Emmett–Teller (BET) method and Barett–Joyner–Halenda (BJH) model, respectively. For the confirmation of the existence of RGO, Raman spectrum was performed by a Raman spectrometer (Thermo Scientific DXR2). Besides, the elemental analyses were performed by X-ray photoelectron spectroscopy (XPS, ESCALAB 250, Al Kα radiation).
Devices Fabrication and Measurement
As-prepared RGO@SiNWs (~ 5 mg) was mixed with ethanol (~ 100 μL), and dispersed uniformly by ultrasonic. The dispersed solution was coated onto a ceramic plate with Pt wires (i.e., heater and measurer), and aged under a voltage of 5 V for 3 days in air. Finally, the prepared devices were measured in a gas sensor analyzer (Winsen WS-30A, China). Formaldehyde was produced by the evaporation of formaldehyde solution (40 wt%) at heating holder in chamber. Ethanol, acetone, ammonia, methanol, xylene, and toluene were produced by pure liquid ethanol, acetone, ammonia, methanol, xylene, and toluene respectively. Response is defined as Ra/Rg, where Ra and Rg are the resistances of the sensor in pure air and in formaldehyde gases. Response/Recovery times are defined as the time needed to change to 90% of the total response.
Results and Discussions
In order to study the morphologies and microstructures, SEM and TEM were performed as shown in Fig. 1. Figure 1a displays the large-scale top view SEM image of as-prepared SiNWs, showing the uniform surface and congregated bundles of SiNWs due to the electrostatic attraction among SiNWs [41, 42]. There are full of large pores with the size of 2~15 μm on the surface as observed in zoomed-in SEM in Fig. 1b. As depicted in the cross-section SEM images of n- and p-SiNWs in Fig. 1c, d, the etched NWs are all perpendicular to the smooth substrate, proving the same <100> orientation as the starting wafer. In addition, the similar length of ~ 24 μm, diameter of 100~300 nm, and density of approximately 1010 cm−2  were demonstrated distinctly, which indicates no difference between <100> oriented n- and p-SiNWs. The scraped n- and p- SiNWs are observed in Additional file 1: Figure S1a and b, which reflect no morphology change after scripting. In order to further confirm the diameter and orientation, TEM images of single n- and p-SiNWs display the diameter of 210 nm (Fig. 1e) and 200 nm (Additional file 1: Figure S2a), respectively. Figure 1f and Additional file 1: Figure S2b are high-resolution TEM (HRTEM) images together with the Fast Fourier Transfer (FFT), measuring the single crystalline structure and the <100> crystal orientation with the (200) spacing of 0.27 nm. The underlying mechanism of SiNWs fabrications using metal-assisted chemical etching (MACE) method is a series of simple redox reactions with the help of Ag catalysts, which can be described briefly by Eq. 1 and Eq. 2.
Reaction at metal (i.e., Ag particles):
Reaction at Si substrate:
Throughout this process, Ag nanoparticles directly seize electrons from Si because of the higher electronegativity of Ag compared with Si, creating a hole-rich region around the Ag nanoparticles. Then, H2O2 is reduced by Ag nanoparticles and Si is oxidized to be SiO2, which is dissolved quickly by HF solution .
Next, the as-etched SiNWs were functionalized by RGO. Figure 1g is the SEM image of RGO@n-SiNWs and Fig. 1h is the zoomed SEM images of RGO@n-SiNWs, which proved that RGO was compactly and uniformly wrapped on the surface of NWs. There would be a formation of p-n junction between RGO and SiNWs, which is important for the enhancement of sensors sensitivity discussed in the following sections.
To shed light on the components and crystallinity, X-ray diffraction (XRD) patterns are performed as shown in Fig. 2a. For n- and p-SiNWs, the main peaks locate at 28.4°, 47.3°, 56.1°, 69.1°, 76.4°, and 88.0°, corresponding to (111), (200), (400), (331), and (422) planes of cubic silicon structure (JCPDS No. 27-1402), respectively. There was no impurity peak observed, indicating the purity of the samples. The XRD pattern of RGO@n-SiNWs also exhibits the same peaks. Obviously, it is found that the peak intensities of RGO@n-SiNWs declined distinctly, which was attributed to the existence of outer amorphous RGO. In order to confirm that GO was entirely reduced to RGO, the zoomed-in XRD spectra from 10° to 25° were shown in Fig. 2b, which demonstrates a peak of RGO@n-SiNWs located at about 22°, contributable to the reduction of GO to RGO .
In an effort to investigate the sensitivity of RGO@SiNWs to HCHO and the optimal device operation temperature, numerous devices based on SiNWs and RGO@ SiNWs were tested at various temperatures. As displayed in Fig. 3a, b, the response of pristine n-SiNWs is higher than that of p-SiNWs. All the devices based on n-SiNWs and RGO@n-SiNWs show the highest response of 2.5 and 6.4 to 10 ppm at 300 °C. In order to evaluate the dynamic response to various gas concentrations based on n-SiNWs and RGO@n-SiNWs in short time, the dynamic test toward HCHO from 0.1 to 10 ppm at 300 °C was performed as displayed in Fig. 3c. It is distinctly observed that the response of n-SiNWs was increased remarkably by wrapping RGO. Meanwhile, the device based on RGO@n-SiNWs has an outstanding response of 2.4 even at a low-concentration of 0.1 ppm, absolutely meeting the criteria of HCHO. As depicted in non-linear fitting in Fig. 3d, the application limitation (Ra/Rg = 2) was obtained to be 35 ppb, indicating a very low detectable concentration.
Response speed and selectivity are always the important parameters for the practical applications of prepared devices. As indicated in Fig. 4a, both n-SiNWs and RGO@n-SiNWs show extremely short response time (11 and 13 s, respectively), suggesting a relatively fast response. With the purpose to evaluate the selectivity of as-prepared RGO@n-SiNWs sensors, another six typical VOCs (i.e., ethanol, acetone, ammonia, methanol, xylene, and toluene) were employed to examine the sensor selectivity, and the measured results are shown in Fig. 4b, revealing a limited interference to the HCHO detection. The high selectivity to HCHO is resulted by the higher reducibility of HCHO than acetone, ethanol, methanol, toluene, and xylene, as investigated in previous reports [45,46,47]. Thus, HCHO is more easily oxidized by RGO@n-SiNWs, causing the large decreased resistance. Besides, it is noted that there is almost no response to ammonia for Si sensors , because it is not easily oxidized by Si. Apart from selectivity, stability is also a critical challenge in the field of HCHO detection. As investigated in Fig. 5, the response of RGO@n-SiNWs sensors operated at 300 °C changes a little (< 5%) from initial 6.4 to 6.1 after 6 days, indicating an excellent air stability.
The surface-volume ratio (specific surface area) is of great significance to affect gas sensitivity. As studied in nitrogen adsorption-desorption isotherms in Fig. 6a, the surface area is increased from 37.3 m2 g−1 of n-SiNWs to 74.5 m2 g−1 of RGO@n-SiNWs, which was originated from the large surface area of RGO. The enlarged specific surface is bound to increase the effective contact-area between targeted gases and samples, thus further improve gas sensitivity. As presented in Raman spectra (Fig. 6b), correlative peaks of Si displayed at 500 and 912 cm−1 were observed in RGO@n-SiNWs, demonstrating the presence of Si-Si bonds . Besides, peaks at 1390 and 1590 cm−1 are assigned to the D- and G-band peaks of carbon phase due to the disordered and ordered sp2 bonded carbon, respectively , which can infer the presence of reduced graphene oxide. Generally, the ID/IG (the intensity ratio of D and G band) is considered as the most important parameter to evaluate the graphitization degree of carbonaceous materials . The ID/IG is calculated to be 0.72 for RGO@n-SiNWs from Fig. 6b, indicating the high carbonaceous degree of RGO@n-SiNWs.
Besides, the chemical compositions of the RGO-SiNWs composites and pristine SiNWs were evaluated by X-ray photoelectron spectroscopy (XPS). As observed in the high-resolution XPS in the vicinity of Si 2p peaks in Fig. 7a, the Si 2p peak intensity of n-SiNWs is decreased distinctly after coating RGO on their surface, while the corresponding C1s peaks intensity of RGO@SiNWs is also enlarged remarkably by comparison with pure SiNWs as observed in Fig. 7b. All of these analyses further prove that the RGO is successfully coated on the surface of SiNWs. Significantly, an evident left shift toward high energy level is revealed in Fig. 7a, resulted by the electron transfer from SiNWs to RGO. XPS data containing the peak position, peak area, surface atomic ratio is demonstrated in Additional file 1: Table S1. The XPS spectra analysis can verify the formation of p-n junction between RGO and SiNWs, which would enhance the transport of electrons generated through the process of HCHO decomposition, and further facilitate the HCHO sensitivity.
In an attempt to understand the gas sensing characteristics of RGO@n-SiNWs, the mechanism of the detection toward HCHO is schematically demonstrated. When the as-fabricated sensors were exposed to pure air, the resistance (Ra) will be large due to the chemisorption of oxygen trapping electrons from the material and forming a surface depletion region shown in Eq. (3). While the sensors are exposed to HCHO, the HCHO gas will react with O− and O2−, and release electrons to RGO@n-SiNWs, leading to the decrease of resistance (Rg). The reaction process was depicted in Eq. (4) and Fig. 8a.
Finally, the mechanism of sensitivity enhancement induced by the combination of n-SiNWs and RGO was discussed. The combination of RGO and n-SiNWs can form a p-n junction, as a result of the p-type characterization of RGO with a narrow band gap (0.2 eV~2 eV) . This p-n junction formed between SiNWs and RGO has been reported in many previous reports . To understand how this p-n junction improve the sensitivity, the schematic diagram of band structure is described in Fig. 8b. As illustrated in band structure diagram in Fig. 8b, the electrons are transferred from SiNWs and stored in RGO, forming a depletion layer and a built-in electric field. The electron depletion and built-in voltage would enhance the chemical reaction in Eq. (4) and facilitate the electron transfer, thus enhances the gas sensing performance.
In summary, SiNWs with high specific surface area are prepared via metal-assisted chemical etching method (MACE), and then are wrapped by reduced graphene oxide (RGO) to form a p-n junction. After wrapping RGO, the specific surface area increases by 1× demonstrated by N2 absorption-desorption isotherm. More importantly, due to the formed p-n junction, the RGO@n-SiNWs reveals an outstanding sensitivity and high selectivity toward low concentration HCHO at 300 °C. The response of RGO@n-SiNWs increases about 2× toward 10 ppm HCHO (~ 6.4) at 300 °C than that of pristine n-SiNWs (~ 2.5). The application detection limitation can reach 35 ppb (Ra/Rg = 2) obtained by non-linear fitting absolutely meeting the safe standard of indoor air. These results provide a promising possibility to precisely detect the low-concentration HCHO, enabling the monitoring the indoor environment.
High-resolution transmission electron microscopy
International Agency for Research on Cancer
Metal-assisted chemical etching
National Institute for Occupational Safety and Health
Reduced graphene oxide
Reduced graphene oxide-coated n-type silicon nanowires
Reduced graphene oxide-coated silicon nanowires
Sick building syndrome
Scanning electron microscopy
Transmission electron microscopy
Volatile organic compounds
World Health Organization
X-ray photoelectron spectroscopy
Bunkoed O, Davis F, Kanatharana P, Thavarungkul P, Higson SP (2010) Sol-gel based sensor for selective formaldehyde determination. Anal Chim Acta 659:251–257.
Li Y, Chen N, Deng D, Xing X, Xiao X, Wang Y (2017) Formaldehyde detection: SnO2 microspheres for formaldehyde gas sensor with high sensitivity, fast response/recovery and good selectivity. Sensor. Actuat. B Chem. 238:264–273.
Kawamura K, Kerman K, Fujihara M, Nagatani N, Hashiba T, Tamiya E (2005) Development of a novel hand-held formaldehyde gas sensor for the rapid detection of sick building syndrome. Sensor. Actuat. B Chem. 105:495–501.
Hempeljørgensen A, Kjaergaard SK, Mølhave L, Hudnell KH (1999) Sensory eye irritation in humans exposed to mixtures of volatile organic compounds. Arch Environ Healt 54:416–424.
Nielsen GD, Wolkoff P (2010) Cancer effects of formaldehyde: a proposal for an indoor air guideline value. Arch Toxicol 84:423–446.
Chen T, Liu QJ, Zhou ZL, Wang YD (2008) The fabrication and gas-sensing characteristics of the formaldehyde gas sensors with high sensitivity. Sensor. Actuat. B Chem. 131:301–305.
Chung P, Tzeng C, Ke M, Lee C (2013) Formaldehyde gas sensors: a review. Sensors 13:4468–4484.
Mirzaei A, Leonardi SG, Neri G (2016) Detection of hazardous volatile organic compounds (VOCs) by metal oxide nanostructures-based gas sensors: a review. Ceram Int 42:15119–15141.
Chen EX, Yang H, Zhang J (2014) Zeolitic imidazolate framework as formaldehyde gas sensor. Inorg Chem 53:5411–5413.
Tian H, Fan H, Li M, Ma L (2016) Zeolitic imidazolate framework coated ZnO nanorods as molecular sieving to improve selectivity of formaldehyde gas sensor. ACS Sens 3:243–250.
Sayed SE, Pascual L, Licchelli M, Martinezmañez R, Gil S, Costero AM, Sancenón F (2016) Chromogenic detection of aqueous formaldehyde using functionalized silica nanoparticles. ACS Appl Mater Inter 8:14318.
Salthammer T (2013) Formaldehyde in the ambient atmosphere: from an indoor pollutant to an outdoor pollutant? Angew Chem Int Edit 52:3320–3327.
Lee CY, Chiang CM, Wang YH, Ma RH (2007) A self-heating gas sensor with integrated NiO thin-film for formaldehyde detection. Sensor. Actuat. B Chem. 122:503–510.
Güntner AT, Koren V, Chikkadi K, Righettoni M, Pratsinis SE (2016) E-nose sensing of low-ppb formaldehyde in gas mixtures at high relative humidity for breath screening of lung cancer. ACS sensors 5:528–535.
Jiang X, Li C, Chi Y, Yan J (2010) TG-FTIR study on urea-formaldehyde resin residue during pyrolysis and combustion. J Hazard Mater 173:205–210.
Nageswari A, Mukkanti K (2012) Low-level quantitation of formaldehyde in drug substance by HPLC–UV. Chromatographia 75:275–280.
Korpan YI, Soldatkin OO, Sosovska OF, Klepach HM, Csöregi E, Vocanson F, Jaffrezic-Renault N, Gonchar MV (2010) Formaldehyde-sensitive conductometric sensors based on commercial and recombinant formaldehyde dehydrogenase. Microchim Acta 170:337–344.
Choi SJ, Jang BH, Lee SJ, Min BK, Rothschild A, Kim ID (2014) Selective detection of acetone and hydrogen sulfide for the diagnosis of diabetes and halitosis using SnO2 nanofibers functionalized with reduced graphene oxide nanosheets. ACS Appl. Mater. Inter. 6:2588–2597.
Hui C, Hu J, Li GD, Qian G, Wei C, Zou X (2017) Porous Ga-in bimetallic oxide nanofibers with controllable structures for ultrasensitive and selective detection of formaldehyde. ACS Appl. Mater. Inter. 9:4692–4700.
Chen T, Zhou Z, Wang Y (2009) Effects of calcining temperature on the phase structure and the formaldehyde gas sensing properties of CdO-mixed In2O3. Sensor. Actuat. B Chem. 135:219–223.
Lv P, Tang ZA, Yu J, Zhang FT, Wei GF, Huang ZX, Hu Y (2008) Study on a micro-gas sensor with SnO2 –NiO sensitive film for indoor formaldehyde detection. Sensor. Actuat. B Chem. 132:74–80.
Zheng Y, Wang J, Yao P (2011) Formaldehyde sensing properties of electrospun NiO-doped SnO 2 nanofibers. Sensor. Actuat. B Chem. 156:723–730.
Zeng W, Liu T, Wang Z, Tsukimoto S, Saito M, Ikuhara Y (2009) Selective detection of formaldehyde gas using a Cd-doped TiO2-SnO2 sensor. Sensors 9:9029–9038.
Wang S, Cao J, Cui W, Fan L, Li X, Li D (2018) Oxygen vacancies and grain boundaries potential barriers modulation facilitated formaldehyde gas sensing performances for In2O3 hierarchical architectures. Sensor. Actuat. B Chem. 255:159–165.
Park HJ, Choi NJ, Kang H, Jung MY, Park JW, Kang HP, Lee DS (2014) A ppb-level formaldehyde gas sensor based on CuO nanocubes prepared using a polyol process. Sensor. Actuat. B Chem. 203:282–288.
Kim JY, Choi NJ, Park HJ, Kim J, Lee DS, Song H (2014) A hollow assembly and its three-dimensional network formation of single-crystalline Co3O4 nanoparticles for ultrasensitive formaldehyde gas sensors. JPhys Chem C 118:25994–26002.
Du H, Wang J, Su M, Yao P, Zheng Y, Yu N (2012) Formaldehyde gas sensor based on SnO2 /In2O3 hetero-nanofibers by a modified double jets electrospinning process. Sensor Actuat B Chem 166:746–752.
Chen T, Liu QJ, Zhou ZL, Wang YD (2008) A high sensitivity gas sensor for formaldehyde based on CdO and In2O3 doped nanocrystalline SnO2. Nanotechnology 19:095506(5pp).
Zhou X, Lee S, Xu Z, Yoon J (2015) Recent progress on the development of chemosensors for gases. Chem Rev 115:7944–8000.
Gurlo A (2011) Nanosensors: towards morphological control of gas sensing activity. SnO2, In2O3, ZnO and WO3 case studies. Nanoscale 3:154–165.
Dr MEF, Koplin TJ, Dr USP (2010) Metal and metal oxide nanoparticles in chemiresistors: does the nanoscale matter? Small 2:36–50.
Tricoli A, Righettoni M, Teleki A (2010) Semiconductor gas sensors: dry synthesis and application. Angew. Chem. Int. Edit. 49:7632–7659.
Gong JR (2010) Label-free attomolar detection of proteins using integrated nanoelectronic and electrokinetic devices. Small 8:967.
Sreeprasad TS, Berry V (2013) How do the electrical properties of graphene change with its functionalization. Small 9:341–350.
Shin J, Choi SJ, Lee I, Youn DY, Chong OP, Lee JH, Tuller HL, Kim ID (2013) Thin-wall assembled SnO2 fibers functionalized by catalytic Pt nanoparticles and their superior exhaled-breath-sensing properties for the diagnosis of diabetes. Adv Funct Mater 23:2342–2342.
Zou X, Wang J, Liu X, Wang C, Jiang Y, Wang Y, Xiao X, Ho JC, Li J, Jiang C (2013) Rational design of sub-parts per million specific gas sensors array based on metal nanoparticles decorated nanowire enhancement-mode transistors. Nano Lett 13:3287–3292.
Choi SJ, Chattopadhyay S, Kim JJ, Kim SJ, Tuller HL, Rutledge GC, Kim ID (2015) Coaxial electrospinning of WO3 nanotubes functionalized with bio-inspired Pd catalysts and their superior hydrogen sensing performance. Nanoscale 8:9159–9166.
Deng S, Tjoa V, Fan HM, Tan HR, Sayle DC, Olivo M, Mhaisalkar S, Wei J, Sow CH (2012) Reduced graphene oxide conjugated Cu2O nanowire mesocrystals for high-performance NO2 gas sensor. J Am Chem Soc 134:4905–4917.
Lin Q, Li Y, Yang M (2012) Tin oxide/graphene composite fabricated via a hydrothermal method for gas sensors working at room temperature. Sensor. Actuat. B Chem. 173:139–147.
Xie J, Tong L, Su L, Wang L, Wang Y (2017) Core-shell yolk-shell Si@C@Void@C nanohybrids as advanced lithium ion battery anodes with good electronic conductivity and corrosion resistance. J Power Sources 342:529–536.
Song LF, Luo LQ, Song JJ, Zhang HC, Li X, Cheng SL, Jin W, Tang J, Liu L, Wang FY (2017) Enhanced photodegradation activity of hydrogen-terminated Si nanowires arrays with different-oriented crystal phases. Catalysts 371:1–12.
Wang FY, Yang QD, Xu G, Lei NY, Tsang YK, Wong NB, Ho JC (2011) Highly active and enhanced photocatalytic silicon nanowire arrays. Nanoscale 3:3269–3276.
Li M, Li Y, Liu W, Yue L, Li R, Luo Y, Trevor M, Jiang B, Bai F, Fu P, Zhao Y, Shen C, Mbengue JM (2016) Metal-assisted chemical etching for designable monocrystalline silicon nanostructure. Mater Res Bull 76:436–449.
Stobinski L, Lesiak B, Malolepszy A, Mazurkiewicz M, Mierzwa B, Zemek J, Jiricek P, Bieloshapka I (2014) Graphene oxide and reduced graphene oxide studied by the XRD, TEM and electron spectroscopy methods. J Electron Spectr Osc 195:145–154.
Shewale PS, Yu YS, Kim JH, Bobade CR, Uplane MD (2015) H2S gas sensitive Sn-doped ZnO thin films: synthesis andcharacterizationP. J Anal Appl Pyrol 112:348–356.
Han N, Wu XF, Zhang DW, Shen GL, Liu HD, Chen YF (2011) CdO activated Sn-doped ZnO for highly sensitive, selective and stable formaldehyde sensor. Sens Actuat B :Chem 152:324–329.
Li F, Guo SJ, Shen JL, Shen L, Sun DM, Wang B, Chen Y, Ruan SP (2017) Xylene gas sensor based on Au-loaded WO3·H2O nanocubes withenhanced sensing performance. Sens. Actuat. B :Chem. 238:364–373.
Dwivedi P, Chauhan N, Vivekanandan P, Das S, Kumar DS, Dhanekar S (2017) Scalable fabrication of prototype sensor for selective and sub-ppm level ethanol sensing based on TiO2 nanotubes decorated porous silicon. Sensor. Actuat. B Chem. 249:602–610.
Tao H, Fan L, Song W, Wu M, He X, Qu X (2014) Hollow core–shell structured Si/C nanocomposites as high-performance anode materials for lithiumion batteries. Nanocale 6:3138–3142.
Fan GF, Zhu HW, Wang KL, Wei JQ, Li XM, Shu QK, Guo N, Wai DH (2011) Graphene/silicon nanowire Schottky junction for enhanced light harvesting, ACS Appl. Mater Inter 3:721–725.
The work was financially supported by the National Key R&D Program of China (2016YFC0207100), the Natural Science Foundation of Shandong Province, China (ZR2018JL021 and ZR2014EMQ011), and the National Natural Science Foundation of China (51402160 and 51602314). The work was also supported by the Taishan Scholar Program of Shandong Province, China, and the Opening Project of Key Laboratory of Microelectronic Devices and Integrated Technology, Institute of Microelectronics, Chinese Academy of Sciences.
Availability of Data and Materials
The datasets supporting the conclusions of this manuscript are included within the manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. (a) and (b) Scraping n-SiNWs and p-SiNWs, respectively. Figure S2. (a) TEM images of p-SiNWs. (b) HRTEM image of p-SiNWs together with the corresponding FFT. Table S1. XPS data including the peak position, peak area, surface atomic ratio. (DOC 1938 kb)
About this article
Cite this article
Song, L., Luo, L., Xi, Y. et al. Reduced Graphene Oxide-Coated Si Nanowires for Highly Sensitive and Selective Detection of Indoor Formaldehyde. Nanoscale Res Lett 14, 97 (2019) doi:10.1186/s11671-019-2921-2
- Si nanowires
- Reduced graphene oxide